Download presentation

Presentation is loading. Please wait.

Published byLayton Hotchkin Modified about 1 year ago

1
Materials for Civil and Construction Engineers CHAPTER 5Aggregates

2
5.1 Aggregate Sources Natural: natural sand & gravel pits, river rock quarries (crushed) Manufactured & recycled materials: pulverized concrete & asphalt steel mill slag steel slugs expanded shale styrofoam

3
5.2 Geological Classifications Igneous Sedimentary Metamorphic All three classes of rock are used successfully in CE applications. Check physical, chemical, and mechanical properties, supplemented by mineralogical examination. Historical performance in a similar design.

4
5.4 Aggregate Uses Under foundations and pavements Stability Drainage As fillers Portland Cement Concrete 60-75% of volume 80-85% of weight Hot Mix Asphalt 80%-90% of volume 90-96% of weight

5
Aggregate Sizes Coarse aggregate material retained on a sieve with 4.75 mm openings Fine aggregate material passing a sieve with 4.75 mm openings Traditional Maximum aggregate size – the largest sieve size that allows all the aggregates to pass Nominal maximum aggregate size – the first sieve to retain some aggregate, generally less than 10% Superpave Maximum aggregate size – one sieve size larger than the nominal maximum aggregate size Nominal maximum aggregate size – one sieve larger that the first sieve to retain more than 10% of the aggregate 4.75mm 1” #4 sieve = four openings/linear inch

6
Aggregate Mining Quarry Sand from river deposit

7
5.5 Aggregate Properties Shape and texture Soundness Toughness Absorption Specific gravity Strength and modulus Gradation Deleterious materials and cleanness Alkaline reactivity Affinity for asphalt Superpave consensus properties Typical source properties Needed for PCC and HMA mix design

8
Particle Shape & Surface Texture Shape = angular, rounded, flaky, or elongated Flaky and elongated are bad because of easy breakage and difficulty compacting in thin asphalt layers High friction (angular, rough) for strength & stability of asphalt Low friction (rounded, smooth) for workability of concrete

9
Angular Rounded Flaky Elongated Flaky & Elongated

10
Coarse Aggregates Particle Shape Evaluation Shape – Flat and elongated test Flat and elongated device Flat Elongated Flat and Elongated

11
Coarse Aggregates Particle Shape & Surface Texture Evaluation Texture and angularity – fractured faces Visual inspection to determine the percent of aggregates with: no fractured faces one fractured face more than one fractured face

12
Fine Aggregates Particle Shape & Surface Texture Evaluation Fine aggregate <1/4” too small for individual inspection Estimated by determining the uncompacted void content of a sample of aggregate Angular Round Measure mass of aggregates in cylinder, use specific gravity to determine volume of aggregates in container. Compute the percent of voids in the aggregates

13
Soundness & Durability Resist weathering water freezing in voids fractures & disintegrates aggregates Test method uses “salt solution” to simulate freezing Prepare sample minimum mass specified gradation Soak 16 hrs – dry 4 hrs Repeat cycle 5 times Measure gradation

14
Toughness & Abrasion Resistance Resist load damage During construction Traffic loads LA abrasion test Prepare sample Minimum mass original Specified gradation Charge drum w/ sample Steel spheres 500 revolutions Sieve 14

15
Bone dry – dried in oven to constant mass Internal impervious voids Air dry – moisture condition state undefined Saturated surface dry – moisture condition state undefined Moist – moisture condition state undefined Voids partially filled WsWs WmWm W SSD =W s +W p WmWm Free moisture Moisture contentAbsorptionMoisture content Absorption is the moisture content when the aggregates are in the SSD condition Free moisture is the moisture content in excess of the SSD condition. A Percent free moisture = M - A Important for proportioning concrete negative free moisture – aggregates will absorb water positive free moisture – aggregates will release water Aggregate Moisture States

16
Specific Gravity The mass of a material divided by the mass of water whose volume is equal to the volume of the material at a specific temperature, or G = / w w = density of water at specified temperature 4 C, w is: 1000 kg/m 3 = 1 g/ml = 1 g/cc 62.4 lb/ft 3 (remember to stay consistent with force and mass units for measurements and the issue of force and mass will go away as G is a ratio) Mass Solid Volume Mass Water Volume G =

17
Determining Specific Gravity Mass Solid Volume Mass Water Volume Mass Solid Mass Water Mass Solid Mass Water Determine by weighing in air Determine by (weight in air - weight in water)

18
Why Weigh in Water? V = 400 ml M = 400 g + V = 250 ml M = 500 g = V = 650ml M = 900 g - V = 250 ml M = 250 g = V = 400 ml M = 650 g Volume of water = initial water - removed water = = 150ml Mass of water = 150 g (1 g/ml) Total mass = = 650 g Direct solution

19
Why Weigh in Water? Mass in air SG = Mass in air + Mass water - Mass in water V = 400 ml M = 400 g + V = 250 ml M = 500 g = V = 650ml M = 900 g = V = 400 ml M = 650 g - V = 250 ml M = 250 g SG = = = = value from direct solution

20
Effects of Voids Voids on the surface of aggregates create multiple definitions of specific gravity Apparent Bulk, Dry Bulk, SSD

21
Apparent Specific Gravity G sa = Mass, oven dry agg Vol of agg Apparent Functional definition Volume of aggregate Stone

22
Bulk Specific Gravity, Dry G sb = Mass, oven dry Vol of agg. + surface voids Vol. of water-perm. voids Surface Voids Functional definition Bulk Stone

23
Bulk Specific Gravity, ssd (saturated surface dry) G s,b ssd = Mass, SSD Vol of agg. + surface voids Vol. of water-perm. voids Surface Voids Functional definition Bulk, saturated surface dry Stone Used for concrete mix design

24
Effective Specific Gravity Used for hot mix asphalt design G se permeable

25
Coarse Aggregate Specific Gravity by the Book (ASTM C127) Dry then saturate the aggregates Dry to SSD condition and weigh Measure submerged weight Measure dry weight

26
Fine Aggregate Specific Gravity by the Book (ASTM C128) Pycnometer used for FA Specific Gravity

27
Bulk Unit Weight & Voids in Aggregates Previous treatment of specific gravity and unit weight were for aggregate particles. The voids considered were for the voids at the surface of the particles. Sometimes we need to know the mass or weight of aggregate required to fill a volume, e.g. the volume of coarse aggregate in a cubic yard of concrete. Bulk unit weight is the weight of aggregate required to fill a “unit” volume. Typical units are cubic meters and cubic feet.

28
Procedure Aggregate Bulk Unit Weight Loose Shovel dry aggregate into container Limit drop < 2” above rim of container Strike off aggregate level with top of container Determine weight of aggregate in container, W S Compute unit weight Compacted Shovel dry aggregate into container Fill to 1/3 of volume Rod 25 times Repeat 3x to fill container Strike off aggregate level with top of container Determine weight of aggregate in container, W S Compute unit weight

29
Strength & Modulus Strength of concrete or asphalt cannot exceed strength of aggregates Typical compressive strength of 5, ,000 psi test parent rock like concrete cylinders but 1.5“ - 2.5" diameter cores from hollow core drill test bulk aggregates in triaxial cell Resilient Modulus Test M R = resilient (recoverable) deformations not permanent deformations M R = resilient (recoverable) deformations not permanent deformations

30
Aggregate Gradation

31
Aggregate Sizes (Review) Coarse aggregate material retained on a sieve with 4.75 mm openings Fine aggregate material passing a sieve with 4.75 mm openings Traditional Maximum aggregate size – the largest sieve size that allows all the aggregates to pass Nominal maximum aggregate size – the first sieve to retain some aggregate, generally less than 10% Superpave Maximum aggregate size – one sieve size larger than the nominal maximum aggregate size Nominal maximum aggregate size – one sieve larger that the first sieve to retain more than 10% of the aggregate 4.75mm 1” #4 sieve = four openings/linear inch

32
Semi Log Graph

33
Types of Gradation Maximum Density Gradation: 0.45 Power Chart High density gradation (Well Graded) has a good mix of all particle sizes which means the aggregates use most of the volume and less cement or asphalt is needed One-size gradation (Uniform) all same size = nearly vertical curve Gap-graded missing some sizes = nearly horizontal section of curve Open-Graded missing small aggregates which fill in holes between larger ones lower part of curve is skewed toward large sizes

34
Sieve Size Percent Passing Straight line identifies maximum density aggregate blend But a special scale is needed for the size axis 0.45 Power Graph

35
Types of Gradation on 0.45 Power Graph

36
This blend of aggregates results in the maximum weight of aggregates that can be placed in a container.

37
ASTM Gradation Specifications Concrete coarse aggregates Size specified by “gradation number” N xy N gradation size number small N = large aggregates range 1 to 8 xy = modifiers for the gradation size. SievePercent Passing 9.5 mm (3/8) mm (No. 4)95– mm (No. 8)80– mm (No. 16)50– mm (No. 30)25– mm (No. 50)10– mm (No. 100)2–10 Concrete fine aggregate control points Control points – the range of allowable percent passing for each “control” sieve

38
AASHTO Gradation Specifications For Superpave (hot mix asphalt) Sieve Size, mm (in.) Nominal Maximum Size (mm) (2 in.)100————— 37.5 (1 1/2 in.) 90–100100———— 25 (1 in.)90 max90–100100——— 19 (3/4 in.)—90 max90–100100—— 12.5 (1/2 in.)——90 max90– (3/8 in.)———90 max90–10095– (No. 4)————90 max90– (No. 8)15–4119–4523–4928–5832–67— 1.18 (No. 16)—————30– (No. 200) 0.0–6.01.0–7.02.0–8.02.0– –12.0 Mix types – identified by nominal max agg size Five control points per mix type

39
Fineness Modulus a measure of the gradation fineness used for Concrete mix design daily quality control for concrete mix design R i = cumulative percent retained on sieve sequence #100, 50, 30, 16, 8, 4, and 3/8“ sieves range of for fine aggregate types larger FM being coarser aggregate

40
Blending Aggregate Gradations Stockpile aggregates with limited size range controls segregation – determine blend of stockpiles to meet required control points. Trial & Error Method P i = A i a + B i b + C i c…. For sieve size i, Pi = percent in the blend that passes sieve size i A i, B i, C i … = percent of each stockpile in the blend a, b, c … = percent of stockpile A, B, C that passes sieve size i Use spreadsheet program for trial and error calculations

41
Properties of Blended Aggregates Blended specific gravity: Other properties weighted average:

42
Cleanness and Deleterious Materials Deleterious Substances Organic impurities Minus mm (No. 200) Coal, lignite, or other low density materials Clay lumps and friable particles Soft particles Sand Equivalency Test SE = h sand / h clay x 100

43
Alkali- Aggregate Reactivity Silica in some agg. reacts with the alkalis (Na 2 O, K 2 O) in Portland Cement (especially in warm, humid climates) excessive expansion cracking popouts Carbonates in aggregate can also react to a lesser extent Minimizing reactivity if a reactive aggregate must be used Type II cement – minimizes alkali content of P.C. Keep concrete as dry as possible Fly Ash (Pozzolans) reduce alkali reactivity (not too much) Sweetening – add crushed limestone to the aggregate

44
Alkali-Aggregate Reactivity Tests ASTM C227 – tests expansion potential of cement-agg. combination expansion of mortar bar at specific temp. & humidity ASTM C289 – reactive silicates in agg. ASTM C586 – reactive carbonates in agg.

45
Asphalt Affinity Affects the bond between asphalt binder and aggregate Asphalt Stripping (moisture induced damage) water causes asphalt film to separate from agg. reduces durability of Asphalt Concrete (A.C.) Hydrophilic (water-loving) silicates – acidic, negative surface charge more susceptible to stripping Hydrophobic (water-hating) limestone – basic, positive surface charge less susceptible to stripping stripping is also affected by porosity, absorption, coatings, etc. Testing ASTM D1664 & D submerge AC in tepid or boiling water ASTM D1075 – freeze-thaw cycles

46
5.6 Handling Aggregates Minimize segregation, degradation, and contamination Avoiding Segregation separation into components with similar characteristics any movement of aggregates promotes segregation small drop height build stockpiles in multiple cones fractionalize stockpiles close to single size aggregates in each stockpile batch separately Avoiding degradation small drop height

47
Sampling Aggregates Random and representative of entire stockpile sample from entire width of conveyor belts at several locations sample from top, middle, and bottom of stockpile at several locations around stockpile diameter use larger sample for testing larger max. size Sample splitting or quartering to reduce sample size from large stockpile to small 1-5 kg sample Sample Splitter Quartering

Similar presentations

© 2016 SlidePlayer.com Inc.

All rights reserved.

Ads by Google